Nanoparticles are the simplest form of structures with sizes in the nm range. In principle anycollection of atoms bonded together with a structural radius of < 100 nm can be considered a
These can include, e.g., fullerens, metal clusters (agglomerates of metal atoms), large molecules,
such as proteins, and even hydrogen-bonded assemblies of water molecules, which exist in water at
Nanoparticles are very commonplace in nature - for instance proteins exist in almost all biological
systems, metal-oxide nanoparticles are easily produced, etc . . .
Introduction to Nanoscience, 2005 JJ J I II 1
2.1. Physically manufactured nanoparticles
When studying nanoparticles a distinction must neccessarily be made between condensed hard
matter nanoparticles, generally termed nanoclusters, and soft bio-organic nanoparticles and largemolecules.
A nanocluster is a nanometer sized particle made up of equal subunits. These subunits can be
atoms of a single element, molecules or even combinations of atoms of several elements in subunits
with equal stoichiometries (alloys, etc.)
E.g.: Nan, (SF6)n, (H2O)n, (Cu3Au)n, (ClCH3C6H3CO2H)n, (TiO2)n, . . .
The greatest difference arises from the fact that molecules have functionality which directly depends
on the inter-positioning of their atoms, whereas the properties of nanoclusters are solely guided by
the number of subunits they contain.
Introduction to Nanoscience, 2005 JJ J I II 2
For this reason clusters can be seen as an intermediate stage between single atoms/molecules and
In general, the physical properties of materials are dependent on the dimensions of the material in
question its properties (e.g. conductivity, elasticity, etc.) are scaleable with respect to the amount
of atoms in the material.
- scaleable size-regime N
Once the particles are small enough - nanoclusters - these properties vary greatly with every addition
or subtraction of an atom.
- non-scaleable size-regime every atom counts !
2.1.2. Size does matter small is very different!
188.8.131.52. Geometric structure
Usually the crystal structure of a large nanocluster is the same as the bulk structure of the material,
Introduction to Nanoscience, 2005 JJ J I II 3
with somewhat different lattice parameters (in general clusters are slightly contracted as compared
E.g. Cu clusters tend to have an FCC structure (Wulff polyhedra).
Some exceptions do, however, occur. Smaller clusters of Cu (e.g. Cu55, Cu147, . . . ) have perfect
- structural magic numbers: occur when an exact amount of atoms is needed for a specific structure
Even smaller clusters can be amorphous-like (spherical, etc.), although a general tendency of the
clusters is to form structures where the total surface energy (and internal energy) is minimized -
Introduction to Nanoscience, 2005 JJ J I II 4
the exact structure then depends on the surface energies related to the specific crystal facets of the
184.108.40.206. Electronic structure
Structural magic numbers affect the formation and abundancies of larger clusters, whereas for the
case of smaller clusters the combined electronic structure of all the atoms is of greater importance.
For instance in a Pbn cluster spectrum, clusters with n=7 or 10 are more abundant than others.
When the ionization potentials of sodium clusters are plotted as a function of the number of atoms
in the clusters, peaks are observed at clusters having two and eight atoms. This can be compared to
the high ionization potentials observed for example in rare-gas atoms, where electrons are removed
from filled orbitals.
- electronic magic numbers are observed for clusters (although most apparent for small clusters
these magic numbers can be noticed even for very large clusters - up to several thousands of atoms.)
Introduction to Nanoscience, 2005 JJ J I II 5
The jellium model has successfully been used in the theoretical modelling of nanoclusters. Thejellium model envisions a cluster of atoms as a single large atom, where the distribution of ionic
Introduction to Nanoscience, 2005 JJ J I II 6
cores is replaced by a constant positive background, the so called jellium density, and only valence
electrons are treated explicitly.
In effect a large spherically symmetric potential well is used to represent the potential describing
the interaction of valence electrons with the positive spherical charge distribution. Energy levels can
be calculated by solving the Schrodinger equations in a fashion analogous to that for the hydrogen
As can be seen from the jellium model, the electronic structure of a cluster varies from that that of
a single atom, but it also varies greatly from that of a bulk material. When a bulk lattice is formed,
Introduction to Nanoscience, 2005 JJ J I II 7
the discrete energy levels of the atoms are smuged out into energy bands. E.g. valence bands and
conduction bands exist in semiconductors and metals. As particles shrink in size there is a dramatic
change in these bands, as the continuous density of states in bulk is replaced with a set of discrete
220.127.116.11. Optical properties
This leads to interesting optical properties. In semiconductors the band gap will be increased ascluster size is decreased a blue shift in the absorption spectrum of the semiconductor (good for
Individual energy levels and enrgy level seperations are also dependent on the size of the clusters,
Introduction to Nanoscience, 2005 JJ J I II 8
which therefore affect the enrgies needed for the transitions of electrons to excited states. Clusters
of different sizes will therefore have different absorption spectra and hence different colours!
Since the electronic structure of nanoclusters depends on their size, their ability to react withother species should also depend on size. This has important applications for the design of catalytic
Introduction to Nanoscience, 2005 JJ J I II 9
Reactivity is highly dependent on the electronic structure, leading to large variations in the reactivity
of clusters even with sizes differing by only single atoms. In general, however, the reactivity of all
nanoclusters is high as compared to that of bulk, due to their higher surface to volume ratio. E.g.
gold nanoclusters are highly reactive if compared to the fairly inert bulk material.
18.104.22.168. Melting temperatures
Another effect caused by a high surface to volume ratio in clusters, is a substantially lower melting
temperature as compared to bulk materials. Unusual phenomena such as negative heat capacitieshave also been observed in clusters (at the melting temperature, an increase of the internal energy
of Na+147 by 1 eV leads to a decrease in temperature by about 10 K).
In large enough systems added energy is converted completely into potential energy, reducing
continuously the fraction of its solid phase. The kinetic energy and thus the temperature remain
constant. A small system, on the other hand, tries to avoid partly molten states and prefers to
convert some of its kinetic energy into potential energy instead. Therefore the cluster can become
colder, while its total energy increases.
Introduction to Nanoscience, 2005 JJ J I II 10
22.214.171.124. Magnetic properties
Interesting magnetic properties have also been observed in small clusters. In a cluster the magneticmoment of each atom will interact with the moments of the other atoms, and can force all the
moments to align in one direction with respect to some symmetry axis of the cluster the cluster
will have a net magnetic moment, it will be magnetized.
As cluster size decreases it therefore becomes easier for them to exhibit ferromagnetic behaviour.
In some cases, even clusters made up of nonmagnetic atoms can have a net magnetic moment. For
instance rhenium clusters show a pronounced increase in their magnetic moment when they contain
less than 20 atoms. For clusters with less than 15 atoms these moments are fairly large.
Introduction to Nanoscience, 2005 JJ J I II 11
2.1.3. Cluster production
In principle there are three different physical methods for producing clusters. Common for all
methods is the initial vaporization of atoms from a bulk target.
126.96.36.199. Energetic vaporization
Energetic vaporization is the simplest of all cluster production methods. Clusters are the resulting
product of the ejection of large numbers of atoms, at high energies, from the bulk material.
Various different vaporization techniques are used in different sources. Including:
- Laser vaporization sources, where atoms are irradiated with intense laser beams.
- Pulsed-arc sources, where intense electrical discharges cause vaporization.
- Ion sputtering sources, where atoms are ejected from the target through ion bombardment.
- Liquid-metal ion sources, where a needle is wetted with the material, after which a high potential
is applied, causing intense eletrical fields, due to which small droplets of the wetting material are
Clusters produced with these sources are generally rather small and extremely